|Email Newsletters from Pharmaceutical Technology and Pharmaceutical Technology Europe|
News from Europe's pharmaceutical manufacturing industry coupled with upcoming events, and exclusive articles and interviews from industry experts.
Defining the ideal properties of a moisture protective, instant release film coating
Many APIs are moisture-sensitive and thus need protection against ambient moisture. Usually, packaging materials are employed that provide a tight enclosure, but this adds costs to the already expensive manufacturing process. A more cost-effective alternative is to use well-formulated moisture protective coatings that reduce water vapour transmission rate (WVTR).
WVTR can be described using Fick's first law,2 which states that the amount of water vapour diffusing across a film barrier at a given time is a function of the following:
To prevent free diffusion of water molecules across the film membrane, water-insoluble additives, such as pigments, can be incorporated into the coating formulation.4,5
The effect of this is prolonged diffusion time and distance within the core, which helps protect against moisture. A crucial polymer characteristic for this method of moisture protection is the flexibility of the polymer film; it must allow the incorporation of large amounts of water-insoluble pigments without negatively affecting the film strength and flexibility.
Preparing the polymers
To compare the characteristics of different polymers, we first prepared 20% polymer solutions, which were then cast as films on a Coatmaster (Erichsen, Germany) The cast films were left to acclimatise at 23 °C/50% relative humidity (RH)6 for at least 48 h. Film strips with a 4 mm diameter were cut out using a manual punch, care being taken not to transfer moisture from the fingers to the film.
The cross section of the film was calculated based on the film thickness and width to calculate the strain. A self programmed Excel macro was then used to compute values obtained. The following elongation at break values were obtained for the polymers used: HPMC (3cP-grade: 3%; 6cP-grade: 11%), PVA (226%) and Kollicoat Protect (256%).6
Comparing the WVTR of different polymers
One method of determining the effectiveness of a moisture protective coating is by measuring the WVTR of the polymer films.
Moisture protection formulations based on HPMC, (incorporating stearic acid for moisture protection), PVA and Kollicoat Protect were prepared, and cast directly onto a PVC layer placed on a heatable metal plate. Typically, film coating processes are performed with an inlet air temperature of 50–80 °C resulting in product temperatures of 35–45 °C,6,7 so the cast films were dried at 45 °C.
Optimizing the formula
Influence of pigments on WVTR
The effect of pigment concentration and type on WVTR was investigated, by preparing isolated films of the polymer suspension containing different pigments, and determining their WVTR.4 Figure 2 shows that the formulation containing 75% pigment gave the greatest reduction in WVTR.
Further studies however, were performed to assess film flexibility. With a polymer content of 25%, films were found with an elasticity of 1–3%, whereas, higher contents of Kollicoat Protect increased the elasticity of the film to more than 3%. We decided, therefore, to continue our studies with the formulation containing 50% pigment as we found that this gave the best balance between moisture protection and film flexibility (the elongation at break for Kollicoat Protect with a 50:50 ratio was more than 10%).
The 50% polymer suspension was, therefore, selected to assess the effect of pigment shape on WVTR.
Based on their barrier-enhancing properties,7,9,10 the following additives were tested — Myrj 59, Brij 721, stearic acid, carnauba wax, lecithin, xanthan gum, SDS and Aerosil R 972 (Evonik). Our studies showed that some of the additives (e.g., stearic acid, lipophilic Aerosil) increased film brittleness.4 Therefore, only additives that significantly improve the film's moisture barrier function should be used. In our study, we found that the combination of sodium lauryl sulfate and hydrophobic fumed silica, gave the best WVTR with a reduction of 80%.4
The film coating process was investigated for Kollicoat Protect-, PVA- and HPMC-based protective coatings, using the Process-Parameter-Chart.11 This chart is based on the assumption that adjustable process parameters, such as inlet air temperature, humidity and spray rates, will affect the process time.
On plotting the product temperature against the process time, and assigning colour charts based on the aesthetic quality of the coated core, a frame that is used for process comparison of film coating formulations was developed.
The plotted values were assigned colour codes, based on their degree of acceptability: dark green >light green >orange >red, where dark green is the most acceptable coat quality.
The data in Figures 4–6 were obtained for the film coating of 8.5 kg cores to a weight gain of 3.5%.11 An AccelaCoater 24" (Manesty, UK) with a drum speed of 12 rpm was used. Other coating conditions were:
Thorsten Cech is manager of the European Pharma Application Lab at BASF. email@example.com
Maureen Mistry is a Technical Service Manager at BASF Pharma Ingredients & Services Europe. firstname.lastname@example.org
1. J. Bley, J. Siepmann and R. Bodmeier, Int. J. Pharm., 378, 59–65 (2009).
2. S. Yoon, D. Sparks and S. Selke, Pharmacopeial Forum, 35(2), 488–492 (2009).
3. European Medicines Agency (EMEA) — Stability Testing of new Drug Substances and Products, Note for Guidance on Stability Testing: Stability Testing of New Drug Substances and Products, August 2003.
4. T. Agnese and T. Cech, "Developing an Instant release Moisture Protective Coating Formulation based on Kollicoat Protect as Film Forming Polymer," PBP World Meeting (Barcelona, Spain, 7–10 April 2008). www.pharma-solutions.basf.de
5. T.Cech and K.Kolter, "Influence of plasticisers on the film properties of HPMC, and PVA and comparison of the properties of Kollicoat IR as a single film former," Excipient fest Europe (Cork, Ireland, 17–18 June 2008).
6. G. Cole, J. Hogan and M. Aulton, Pharmaceutical Coating Technology, p 199, Taylor & Francis, London, UK (2001).
7. ASTM F-1249 06 Standard Test Method for Water Vapor Transmission Rate Through Plastic Film and Sheeting Using a Modulated Infrared Sensor. www.astm.org/Standards/F1249.htm
8. M.G. Ageeva and E.N. Lazareva, Pharm. Chem. J., 2(10), 582–585 (1968).
9. L.L. Augsburger and Stephen W. Hoag (Third edition, Volume 1), Pharmaceutical Dosage Forms: Tablets (Healthcare USA, Inc. 2008) p 402.
10. T. Cech and K. Kolter, Comparison of the Coating Properties of Instant Release Film Coating Materials Using a Newly Developed Test Method – the Process-Parameter-Chart; PSWC (2007).